Ultra low expansion glass

Ultra low expansion glass (ULE) is a registered trademark of Corning Incorporated. ULE has a very low coefficient of thermal expansion and contains as components silica and less than 10% titanium dioxide. Such high resistance to thermal expansion makes it very resistant to high temperature thermal shock. ULE has been made by Corning since the 1960s,[1] but is still very important to current applications.

## Contents

* 1 Applications
* 2 Structure
* 3 Processing
* 4 Properties
* 4.1 Thermal
* 4.2 Mechanical
* 4.3 Optical
* 4.4 Other
* 5 References

## Applications

Hubble Space Telescope mirror made out of ULE glass.

There are many applications for ULE, but by far the most common is for mirrors and lenses for telescopes in both space and terrestrial settings. One of the most well known examples of the use of ULE is in the Hubble Space Telescope's mirror. Another good example of its application is in the Gemini telescope's mirror bank. This type of material is needed for this application because the mirrors on telescopes, especially very large, high-precision units, cannot bend or lose their shape even slightly. If this were to happen, the telescope would be out of focus.[1] Some other examples and uses of ULE are:

* Ultra-low expansion substrates for mirrors and other optics
* Length standards
* Lightweight honeycomb mirror mounts
* Astronomical telescopes
* Precision measurement technology
* Laser cavities

Another newer use for this material that is showing promise is in the semiconductor industry, this again because of the purity and extreme low expansion of ULE glass.[1]

## Structure

The structure of ULE is completely amorphous; because of this it is a glass, not a ceramic. The amorphous structure of the material comes from there being no crystal phases within the structure, so there is no long range order.

## Processing

Diagram of process of making ULE glass.

The way that ULE is made is very different from the standard way that glass is made. Instead of mixing powdered materials together into a batch, melting that batch and pouring out sheets of glass, ULE, being such a high temperature glass, has to be made in a flame hydrolysis process. In this process high purity precursors are injected into the flames, which causes them to react and form TiO2 and SiO2. The TiO2 and SiO2 then fall down and are deposited onto the growing glass.[1]

## Properties

### Thermal

Ultra low expansion glass has an coefficient of thermal expansion of about 10−8/K at 5–35 °C.[2] It has a thermal conductivity of 1.31 W/(m·°C), thermal diffusion of 0.0079 cm2/s, a mean specific heat of 767 J/(kg·°C), a strain point of 890 °C [1634 °F], and an estimated softening point of 1490 °C [2714 °F], an annealing point of 1000 °C [1832 °F].[3]

### Mechanical

Ultra low expansion glass has an ultimate tensile strength of 49.8 MPa (7,220 psi), a Poisson’s ratio 0.17, a density of 2.21 g/cm3 (0.079 lb/in3), a specific stiffness of 3.12×106 m (1.23×108 in), a shear modulus of 29.0 GPa (4.20×106 psi), a bulk modulus of 34.1 GPa (4.95×106 psi), and an elastic modulus of 67.6 GPa (9.80×106 psi).[3]

### Optical

ULE has a Stress Optical Coefficient of 4.15 (nm/cm)/(kg/cm3) [0.292(nm/cm) psi], and an Abbe number of 53.1.[3]

### Other

ULE has a high resistance to weathering because of its hardness, and is also unaffected by nearly all chemical agents. ULE also shows no changes when quickly cooled from 350 °C.[3]

## References

1. ↑ 1.0 1.1 1.2 1.3 Hrdina, Ken. "Production and Properties of ULE Glass with Regards to EUV Masks". Materials Technology Division. http://www.sematech.org/meetings/archives/litho/euvl/199910XX/108HrdinaULEGlassProduction.pdf.
2. ↑ "ULE Ultra Low Expansion Glass". Specialty Materials. Corning Incorporated. http://www.corning.com/specialtymaterials/products_capabilities/ULE.aspx.
3. ↑ 3.0 3.1 3.2 3.3 "ULE® Corning Code 7972 Ultra Low Expansion Glass". Advanced Optics and Materials. Corning. http://www.corning.com/docs/specialtymaterials/pisheets/ulebro91106.pdf.

* v
* t
* e

Glass science topics

Basics|

* Glass
* Glass transition
* Supercooling

Formulation|

* AgInSbTe
* Bioglass
* Borophosphosilicate glass
* Borosilicate glass
* Ceramic glaze
* Chalcogenide glass
* Cobalt glass
* Cranberry glass
* Crown glass
* Flint glass
* Fluorosilicate glass
* Fused quartz
* GeSbTe
* Gold ruby glass
* Lead glass
* Milk glass
* Phosphosilicate glass
* Photochromic lens glass
* Silicate glass
* Soda–lime glass
* Sodium hexametaphosphate
* Soluble glass
* Tellurite glass
* Thoriated glass
* Ultra low expansion glass
* Uranium glass
* Vitreous enamel
* Wood's glass
* ZBLAN

Glass-ceramics|

* Bioactive glass
* CorningWare
* Glass-ceramic-to-metal seals
* Macor
* Zerodur

Preparation|

* Annealing
* Chemical vapor deposition
* Glass batch calculation
* Glass forming
* Glass melting
* Glass modeling
* Ion implantation
* Liquidus temperature
* Sol-gel technique
* Viscosity
* Vitrification

Optics|

* Achromat
* Dispersion
* Gradient-index optics
* Hydrogen darkening
* Optical amplifier
* Optical fiber
* Optical lens design
* Photochromic lens
* Photosensitive glass
* Refraction
* Transparent materials

Surface
modification|

* Anti-reflective coating
* Chemically strengthened glass
* Corrosion
* Dealkalization
* DNA microarray
* Hydrogen darkening
* Insulated glazing
* Porous glass
* Self-cleaning glass
* Sol-gel technique
* Tempered glass

Diverse
topics|

* Glass-coated wire
* Safety glass
* Glass databases
* Glass electrode
* Glass fiber reinforced concrete
* Glass ionomer cement
* Glass microspheres
* Glass-reinforced plastic
* Glass-to-metal seal
* Porous glass
* Prince Rupert's drops
* Radioactive waste vitrification
* Windshield
* Glass fiber

0.00

(0 votes)

Original source: https://en.wikipedia.org/wiki/Ultra low expansion glass. Read more

|

Retrieved from "https://handwiki.org/wiki/index.php?title=Chemistry:Ultra_low_expansion_glass&oldid=4358921"
*[v]: View this template
*[t]: Discuss this template
*[e]: Edit this template